Composite Laminate Modeling


 Walter Osborne
 1 years ago
 Views:
Transcription
1 omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer
2 WHAT THIS WHITE PAPER OVERS This note is intended for new engineers interested in modeling composites and experienced engineers who would like to get acquainted with the Femap interface. This note is intended to accompany a technical seminar and will provide you a starting background on composites. The following topics are covered: o A little background on the mechanics of composites and how micromechanics can be leveraged to obtain composite material properties o 2D composite laminate modeling Defining a material model, layup, property card and material angles Symmetric vs. unsymmetric laminate and why this is important Results post processing o 3D composite laminate modeling Defining a material model, layup, property card and ply/stack orientation When is a 3D model preferred over a 2D model o Modeling a sandwich composite Methods of modeling a sandwich composite 3D vs. 2D sandwich composite models and their pros and cons o Failure modeling of a 2D composite laminate Defining a laminate failure model Post processing laminate and lamina failure indices Predictive Engineering Document, Feel Free to Share With Your olleagues Page 2 of 66
3 TABLE OF ONTENTS 1. INTRODUTION TERMINOLOGY TYPES OF MATERIALS Anisotropic Material Orthotropic Material Isotropic Material OMPOSITE MIROMEHANIS RULE OF MIXTURES Application Example LAMINATE MODELING IN FEMAP IMPORTANT ENTITIES DEFINING AN ORTHOTROPI MATERIAL UNDERSTANDING THE LAYUP EDITOR PROPERTY ARD: 2D LAMINATE MODELING ASSIGNING MATERIAL ANGLES Defining a Material Angle on the Element Defining a Material Angle in the Property ard Advanced Application Example of Assigning Material Angle to a omplex Geometry PROPERTY ARD: 3D LAMINATE MODELING MULTIMATERIAL ANGLE EXAMPLE OF A 3D OMPOSITE MODEL EXAMPLE 1: REATING A 2D LAMINATE MODEL IN FEMAP INTRODUTION...28 Predictive Engineering Document, Feel Free to Share With Your olleagues Page 3 of 66
4 4.2 REATING THE MATERIAL PROPERTY DEFINING THE LAYUP DEFINING THE LAMINATE PROPERTY (POMP) SPEIFYING MATERIAL ANGLES ANALYSIS SETUP AND POST PROESSING Analysis Set Manager Setup for omposites Post Processing the Results EXAMPLE 2: REATING A 3D LAMINATE MODEL IN FEMAP INTRODUTION REATING THE MATERIAL PROPERTY DEFINING THE LAYUP DEFINING THE LAMINATE PROPERTY (POMPS) SPEIFYING MATERIAL ANGLES POST PROESSING THE RESULTS EXAMPLE 3: MODELING A SANDWIH OMPOSITE INTRODUTION REATING THE MATERIAL PROPERTY DEFINING THE LAYUP DEFINING THE PROPERTY ARDS POST PROESSING THE RESULTS OTHER METHODS FOR SANDWIH OMPOSITE MODELING LAMINATE FAILURE THEORIES IN FEMAP INTRODUTION HILL S THEORY...47 Predictive Engineering Document, Feel Free to Share With Your olleagues Page 4 of 66
5 7.3 HOFFMAN S THEORY TSAIWU THEORY MAXIMUM STRAIN THEORY ONSET FAILURE THEORY EXAMPLE 4: MODELING THE FAILURE BEHAVIOR OF OMPOSITE LAMINATES REATING THE MATERIAL PROPERTY DEFINING THE LAMINATE PROPERTY RESULTS ADDITIONAL READING MATERIAL DATABASE APPENDIX LASSIAL LAMINATION THEORY Kinematic Equations onstitutive Equations Resultants Equilibrium Equations Stiffness Matrices A, B, and D UNSYMMETRI LAYUP HAMIS MODEL ONSET FAILURE THEORY...64 Predictive Engineering Document, Feel Free to Share With Your olleagues Page 5 of 66
6 1. INTRODUTION omposite Laminate Modeling Using Femap 1.1 TERMINOLOGY omposite material: A combination of two or more materials to form a new material system with enhanced material properties. Examples of reinforcements are glass fibers, carbon fibers, silicon carbide fibers etc. Examples of matrix materials are epoxy, polyurethane, silicon carbide etc. Lamina: A lamina is a thin layer of composite material. The thickness of the lamina is usually.1 to 1 mm. It is also referred to as a ply. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 6 of 66
7 Laminate: A laminate is constructed by stacking a number of laminae. The building block for a laminate is lamina. 1.2 TYPES OF MATERIALS In engineering applications, materials can be broadly classified as anisotropic, orthotropic, and isotropic. An anisotropic material has the generalized formulation, while other two are derived by some simplifications ANISOTROPI MATERIAL An anisotropic material has no planes of material symmetry. Examples of anisotropic materials are femur, shortfiber composites etc. The number of constants required to describe anisotropic materials is 21. The stiffness matrix shown below is symmetric about the diagonal terms. Accordingly, all the diagonal terms and the terms above/below the diagonal terms have to be defined in the material model. σ σ σ τ τ τ ε ε ε γ γ γ Predictive Engineering Document, Feel Free to Share With Your olleagues Page 7 of 66
8 Predictive Engineering Document, Feel Free to Share With Your olleagues Page 8 of 66 ORTHOTROPI MATERIAL An orthotropic material has three planes of material symmetry. Examples of orthotropic materials are wood, unidirectional lamina etc. The number of constants required to describe orthotropic materials is 9. The stiffness matrix is symmetric and all the diagonal terms and terms above/below the diagonal terms have to be defined. However, commercial finite element software allow defining the elastic moduli (E 1, E 2, E 3 ), shear moduli (G 12, G 13, G 23 ), and Poisson s ratio (ν 12, ν 13, ν 23 ) instead of calculating each of the stiffness terms. The finite element software can internally evaluate these stiffness terms. ISOTROPI MATERIAL All planes are planes of symmetry. Examples of isotropic materials are metals like steel, aluminum etc. There are only 2 independent constants ( 11 and 12 ) for an isotropic material. Similar to the orthotropic material model, one can define E and ν instead of calculating the stiffness terms. γ γ γ ε ε ε τ τ τ σ σ σ γ γ γ ε ε ε τ τ τ σ σ σ
9 2. OMPOSITE MIROMEHANIS Study of composite material behavior wherein the interaction of constituent materials are examined on a microscopic scale to determine their effect on the properties of the composite material. Predict the properties of composite, given the component properties and their geometric arrangement. The mechanical properties of the composite depend on the percentages of fibers and matrix. 2.1 RULE OF MIXTURES If the fiber and matrix properties are available, a reasonable estimation of the lamina properties can be obtained using the rule of mixtures (strength of materials approach). Here, E L and E T correspond to longitudinal and transverse moduli of the composite lamina, G LT and ν LT correspond to inplane shear modulus and Poisson s ratio, respectively. Suffix f corresponds to fiber property and m corresponds to matrix property. In the above equations, V corresponds to volume fraction APPLIATION EXAMPLE E L 1 E ν T 1 G E V E V LT LT f Vf E We will consider the mechanical properties of a carbon fiber and an epoxy resin to apply the rule of mixtures and estimate the lamina mechanical properties. For this example, we will consider a fiber volume fraction of 56%. For most structural applications, a fiber volume fraction greater than 55% is typically used. Increasing the fiber volume fraction can favor in terms of the load carrying capacity as fibers take majority of the load. However, fiber volume fraction cannot be increased beyond a certain limit (typically around 65%). Just as a note, the theoretical maximum volume fraction for a fiber (cylinder) is 78% for square packing. As the resin content is reduced, fibers are not f f f f Vf G V E f m m m V G m m m m ν V ν V m Predictive Engineering Document, Feel Free to Share With Your olleagues Page 9 of 66
10 completely wet during the manufacturing process and can result in increased dry spots (part quality is reduced). This will result in reduced load transfer between the fibers. onstituent E L (GPa) E T (GPa) ν G (GPa) V f (%) arbon fiber Epoxy resin The carbon/epoxy lamina properties are calculated using the rule of mixtures as shown below. E L = 22* *.44 = 125 GPa 1/ E T = (.56/22) + (.44/3.3) =.14 GPa > E T = 7.4 GPa 1/ G LT = (.56/25) + (.44/1.2) =.39 GPa > G LT = 2.6 GPa ν LT =.56* *.37 =.25 The mechanical properties (2D orthotropic) obtained using the rule of mixtures for a carbon/epoxy lamina are shown below. arbon/epoxy lamina E L (GPa) E T (GPa) G LT (GPa) ν LT Rule of mixtures hamis model Experimental [1] Predictive Engineering Document, Feel Free to Share With Your olleagues Page 1 of 66
11 3. LAMINATE MODELING IN FEMAP In this section, we provide details on modeling composite laminates in Femap. There are four important entities in which modeling laminates differs from conventional metallic components. omposite laminate modeling deals with the following modifications: an orthotropic/anisotropic (typically) material configuration laminates have a layered configuration, so a layup configuration has to be specified with the thickness of each layer and their orientation angles w.r.t a reference axis an element/property type that accounts for the layered configuration has to be used reference axis (material angle) specification Each of the above entities and their definition in Femap is summarized in the following subsections. There are two work flows that can be followed to model a laminate in Femap depending on whether the laminate model is a 2D or 3D. Defining the material cards, layup, and property cards is common between 2D and 3D models; however, material angles can be specified using two approaches in a 2D model while only one approach is used for a 3D model. In 2D models material angles can be specified at element level or directly in the property cards. Specifying material angles on elements is a convenient approach especially for complex geometries; we can select a set of elements and apply the material angle instead of assigning a specific material angle to all elements in a property card. For 3D models, we have to define material angles in the property card and so we need to create multiple property cards for complex geometries. In the following subsections, an overview of Femap interface for laminate modeling is provided accompanied by worked examples. Work flow 1 Work flow 2 laminate (2D) material model layup property card define material angle on element laminate (2D) and solid laminate (3D) material model layup property card with material angle Predictive Engineering Document, Feel Free to Share With Your olleagues Page 11 of 66
12 3.1 IMPORTANT ENTITIES Modeling composites can be easier if the following entities are carefully assigned. It is important to select/create a coordinate system that is appropriate for your composite laminate. In most cases, the basic rectangular coordinate system will work. However, one needs to be careful while dealing with curved laminates. Individual ply orientations assigned in layup editor will be referenced/relative to coordinate system assigned in this step. A material type for the composite laminate should be assigned. Typically used material types are 2D/3D orthotropic materials for continuous fiberreinforced composite laminates. A property card corresponding to a composite laminate has to be specified. For 2D modeling, the element/property type can be a laminate type. Similarly, for 3D modeling, the element/property type can be a solid laminate type. A suitable failure criterion can also be specified using the property card. The composite laminate layup configuration is provided using the layup editor. Using the layup editor, ply stacking (number and direction), ply material, individual ply orientations and ply thicknesses are provided. *Always check your units Predictive Engineering Document, Feel Free to Share With Your olleagues Page 12 of 66
13 3.2 DEFINING AN ORTHOTROPI MATERIAL Notice that we have different properties in longitudinal (E 1 ) and transverse (E 2 ) directions, where E 1 is aligned to the angle specified within the layup. Depending on the type of analysis, various material properties are required. Select an appropriate material type (eg., orthotropic 2D) Required if TsaiWu failure criterion is used. This value is to be experimentally determined. *Always check your units If you have fiber and matrix properties, you can still estimate the composite properties using rule of mixtures or other methods. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 13 of 66
14 3.3 UNDERSTANDING THE LAYUP EDITOR Thickness of individual ply Notice the layup direction (numbering): bottom layer to top layer omputes laminate equivalent properties (inplane properties, bending properties, ABD matrices) Material assigned for each ply in the laminate. Multiple materials can also be assigned (eg., honeycomb core). These angles/orientations are relative to the material angle (reference axis) specified for the element. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 14 of 66
15 Layup viewer is a useful tool to visualize the layup that has been created. It is important to notice that these angles/orientations are relative to the material angle (specified in the property card or on the elements). To avoid confusion, one can draw the orientations along with the assigned material angle and verify if the angles match the actual orientations in your layup. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 15 of 66
16 3.4 PROPERTY ARD: 2D LAMINATE MODELING Default is .5*total thickness Select the layup created 2D laminate modeling Required if a failure criterion is selected. This allowable stress corresponds to interlaminar shear stress. Use a specific failure theory, if you want to compute failure indices of individual plies Explore these options. If all the plies in the laminate are specified in the layup, you can leave it to default. If only half the plies are specified, you can use symmetric option to create a symmetric laminate. Assign an appropriate material angle. Layup angles will be oriented relative to this material angle. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 16 of 66
17 Orientation angles specified in the layup editor Predictive Engineering Femap White Paper 3.5 ASSIGNING MATERIAL ANGLES Although, orientation angles are specified for each lamina individually in the layup editor, Femap will not understand as to which reference direction these orientations (angles) correspond. So, we need to specify a material angle such that all orientations (specified in layup) take this vector as the reference. For example, if the material angle is defined in the global xdirection then all the orientations will use global xdirection as the reference. One should not be confused with the terminologies material angle and orientation angle in the layup editor. Material angle is a reference axis that we assign to the element and is independent of the shape of the element. Orientation angle is the orientation of the lamina (fiber direction). By default, Femap assigns no material angle. Use any of the following methods to specify the material angle. Image source: Predictive Engineering Document, Feel Free to Share With Your olleagues Page 17 of 66
18 3.5.1 DEFINING A MATERIAL ANGLE ON THE ELEMENT One can define/update the material angles using toolbar Modify > Update Elements  > Material Orientation. This method allows one to define a material angle to a selected set of elements or all the elements at a time. It is important to note that the material angle is independent of the element coordinate system and the element shape. For example, the image below shows elements that are distorted. However, the material angles are all aligned to the globalx direction. If a material angle is not defined, Femap will show an error message. If you miss defining a material angle for a few elements in the model, it can be quite difficult to trace the elements with missing definitions. We have developed an API to filter these elements with missing elements and group them. By accessing this newly created group, one can assign/update the material angles to these elements only. The API is called omposites Material Angle hecker, and can be downloaded from our website at One can verify the material angles in the laminate elements by selecting the following options under F6 or View Options. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 18 of 66
19 3.5.2 DEFINING A MATERIAL ANGLE IN THE PROPERTY ARD In this approach, we can define a material angle directly in the property card. However, this will assign the material angle to all the elements that the property id is associated with. One can also check the assigned material angles and update them (in case of any incorrect material angles) accordingly using the procedure in approach 1. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 19 of 66
20 1 Any of these methods can be used 2 In case of a complex geometry with curved surfaces, material angles can be effectively defined using the cylindrical coordinate system by using the tangent direction if the vector has to follow a curved surface. Always remember to verify your material angles! ADVANED APPLIATION EXAMPLE OF ASSIGNING MATERIAL ANGLE TO A OMPLEX GEOMETRY The example below shows a composite wing leading edge. The material angle needs to follow the curvature of the leading edge. However, we can see from the picture that the vectors (representative of the material angles) do not follow the curvature. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 2 of 66
21 Vectors do not follow the curvature of the leading edge In order to assign the material angle accurately, we can use the cylindrical coordinate system (R, T, Z) instead of a rectangular coordinate system (X, Y, Z). We want to create a new cylindrical coordinate system (instead of an existing cylindrical coordinate system) that will do a better job in accurately assigning the material angles. Follow the steps below to create a new cylindrical coordinate system. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 21 of 66
22 The new coordinate system is shown below. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 22 of 66
23 We will use the procedure detailed in section (Defining a material angle on the element) to update the material angle. Go to toolbar Modify > Update Elements  > Material Orientation. This will prompt you to select the elements for which the material angle has to defined/updated. For this example, we will select all the laminate plate elements. Next, you will be prompted to select the material orientation direction (shown below). The above procedure will orient the all the material angles along the curvature of the leading edge. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 23 of 66
24 3.6 PROPERTY ARD: 3D LAMINATE MODELING For 3D laminate modeling, one can specify both shear stress allowable and normal stress allowable for the bond. 3D laminate modeling Notice that, failure theories are not available in the property card. In solid laminates, failure criterion is specified using the materials card. In 3D laminate modeling, we define a ply/stack direction instead of a material angle. For example, if the material angle is in globalx and the layup stacking in globalz, then we specify the ply/stack direction as XZ (13). Unlike 2D, we cannot use approach 1 (Modify > Update Elements  > Material Orientation) for 3D solid laminate elements. We can create multiple property cards (if necessary) with different ply/stack directions for sections of your geometry. And try to explore other coordinate systems for specifying the ply/stack direction. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 24 of 66
25 Specify elastic properties in general tab Specify failure criterion in ply/bond failure tab 3.7 MULTIMATERIAL ANGLE EXAMPLE OF A 3D OMPOSITE MODEL This example shows a composite component with sections oriented in different directions. The component is modeled using laminate solid elements. Here, we cannot use a single ply/stack direction for all the sections of the component. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 25 of 66
26 In this example, we will create three property cards (identified by color as shown above) to define ply/stack direction separately for each of the three sections of the composite component. The following images will show how ply/stack directions have been defined for these sections. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 26 of 66
27 Predictive Engineering Document, Feel Free to Share With Your olleagues Page 27 of 66
28 4. EXAMPLE 1: REATING A 2D LAMINATE MODEL IN FEMAP 4.1 INTRODUTION In this example, we will analyze a simple composite laminate with a hole subjected to uniaxial tension. omposite laminates are often studied for openhole tension in the aerospace industry. The material, layup, and the thicknesses used in this example are from a real world composite part. Here, we will study two types of layups with the same number of layers and same orientations but stacked in different ways. We will analyze the differences in the results just by altering the layup stacking order. We will learn this unique behavior of composites by working out this example. With multiple plies in the layup, this is also a good example for post processing. 4.2 REATING THE MATERIAL PROPERTY The material properties used for the laminate correspond to a unidirectional carbon/epoxy lamina. Accordingly, the material type needs to be 2D Orthotropic for this problem. The material properties are shown in Table 1. Table 1. Mechanical properties of a unidirectional T8S/392 lamina Property Unit T8S/392 Longitudinal elastic modulus (E 1 ) GPa 147 Transverse elastic moduli (E 2 = E 3 ) GPa 7.58 Inplane shear modulus (G 12 ) = Interlaminar shear modulus (G 13 ) GPa 3.96 Interlaminar shear modulus (G 23 ) GPa 3. Inplane Poisson s ratio (ν 12 ) = Interlaminar Poisson s ratio (ν 13 ).33 Interlaminar Poisson s ratio (v 23 ).38 Longitudinal tensile strength (X t ) = Longitudinal compressive strength (X c ) GPa 2.86 Transverse tensile strength (Y t ) = Transverse compressive strength (Y c ) GPa 1.55 Shear strength (S) GPa.14 Predictive Engineering Document, Feel Free to Share With Your olleagues Page 28 of 66
29 Since the laminate model is 2D, the direction 3 properties can be ignored for this problem. 4.3 DEFINING THE LAYUP We will analyze two types of layups in this model. The idea is to observe how the layup can affect your analysis even if the laminate effectively has the same number of layers, same orientation angles, but stacked up in a different sequence. Layup 1: [45 /9 /45 / ] s with each layer at.195 mm thickness. The subscript s in the layup definition shows that it is symmetric laminate. This implies that the layup configuration is [45 /9 /45 / / /45 /9 /45 ]. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 29 of 66
30 Layup 2: [45 /9 /45 / /45 /9 /45 / ]. Layup 2 has 8 layers as layup 1 except that the layup configuration is no longer symmetric about laminate s midplane. The layup editor with Layup 1 defined is shown below. Layup 2 can be defined in a similar manner by changing the orientation angles. 4.4 DEFINING THE LAMINATE PROPERTY (POMP) The Nastran property card for 2D laminates is POMP. Detailed information on the POMP card is available in the Nastran User Guide. The 2D laminate formulation is based on classical lamination theory. Select the Laminate element/property type in the property card. By default, Femap assigns plate element type for 2D models. The layup defined in the previous step can be assigned in the property card. Since we have defined all the 8 layers in the layup, options is left to its default As Specified in the property card. Alternatively, we can define 4 layers only in the layup and use Symmetric option. However, this option has to be used with caution as it cannot be used for unsymmetric Predictive Engineering Document, Feel Free to Share With Your olleagues Page 3 of 66
31 laminates. Ideally, one can define all the layers in the layup editor unless there are a large number of layers (e.g., thick composite). 4.5 SPEIFYING MATERIAL ANGLES For this problem, we will use global xdirection as our material angle. We can use one of the procedures which were introduced earlier. 4.6 ANALYSIS SETUP AND POST PROESSING For this model, a force of 1 kn is applied on the nodes on one end and fixed constraints are applied on the other end as shown below. To simulate the experimental loading behavior, the 1 kn load is applied on an independent node and this node is rigidly linked to nodes on the right end of the laminate model (shown below). When the load is applied on the independent node, the resulting displacement is translated to the dependent nodes. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 31 of 66
32 The model is ready to be analyzed and is solved for a linear static case. The model is analyzed for the two layups and the deformations observed in both these cases are discussed. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 32 of 66
33 4.6.1 ANALYSIS SET MANAGER SETUP FOR OMPOSITES SROMPS controls the computation and printout of ply strength ratios. When on, ply strength ratios are output for composite elements that have failure indices requested. NOFISR controls the printout of the composite failure indices and strength ratios. When on, the failure indices and strength ratios will not be printed. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 33 of 66
34 4.6.2 POST PROESSING THE RESULTS Initially, the model with the symmetric laminate ([45 /9 /45 / / /45 /9 /45 ]) was analyzed. The total translation in this model is shown below. The deformations are symmetric about the xaxis. Under the applied uniaxial tensile load, deformations were inplane as expected. No outofplane deformations were observed. Next, the model with unsymmetric laminate ([45 /9 /45 / /45 /9 /45 / ]) was analyzed. From the contours (shown below), it can be observed that the deformations were not symmetric about the xaxis. Also, we can now see that the unsymmetric laminate resulted in an outofplane deformation although the loading was uniaxial. Symmetric laminate No outofplane deformations Predictive Engineering Document, Feel Free to Share With Your olleagues Page 34 of 66
35 Unsymmetric laminate with outofplane deformations This kind of behavior is unique in fiberreinforced composite laminates and often not explored due to inherent design challenges. An unsymmetric layup can result in warping of the laminate as early as during the manufacturing process when the laminate is cured at high temperatures. Thus, it is quite challenging to design an unsymmetric laminate to suit a specific loading environment. One practical example of an unsymmetric laminate application is in the forward swept composite wings of the X29 aircraft [2]. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 35 of 66
36 X29 aircraft Photo courtesy of Structural Mechanics orporation If this subject interests you, please see the Appendix. Next, we proceed to stress distributions in the individual plies. For this discussion, we will use the symmetric laminate results. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 36 of 66
37 The stress contour shown above corresponds to the major principal stress in ply 4 ( layer). Similarly, we can plot stress distribution in other layers. Femap has bunch of output options and sometimes it can be difficult to find the same output vector for another ply. There are some custom tools available in Femap which can be effectively used for laminates. For example, we can use the Laminate Prev Ply tool to plot ply 3 Major Principal Stress (provided we have a plot of ply 4 Major Principal Stress) without putting effort in finding the output vector amongst large set of results. This will be particularly useful if you have a large number of layers in the laminate. Some of the tools which are specific to laminates are shown below. These tools can be accessed from ustom Tools > PostProcessing. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 37 of 66
38 If you would like to use these API s frequently, we can create a customized toolbar with these commands. It is easier this way to find a command in the toolbar rather than searching for these commands in the ustom Tools. We have created a video on creating a customized toolbar and can be accessed from 5. EXAMPLE 2: REATING A 3D LAMINATE MODEL IN FEMAP 5.1 INTRODUTION In this example, we will develop a 3D laminate model to analyze a simple composite laminate with a hole subjected to uniaxial tension. This is an extension of example 1 to a 3D laminate model. The goal is to understand the applicability of both the models. The material, layup, thicknesses, and the approach used in this example are same as in the example 1. A major difference between the 2D laminate model and the 3D laminate model is that the former will not take outofplane stresses in to account while the latter will. The 3D laminate models will be useful if you are modeling a composite structure with free edges like holes where the outofplane shear stresses can be important. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 38 of 66
39 5.2 REATING THE MATERIAL PROPERTY Defining the material properties for a 3D laminate model is similar to the 2D model except that the material type is now 3D orthotropic. Accordingly, direction3 properties should also be defined. All the required properties are defined in Table DEFINING THE LAYUP Specifying the layup configuration is similar to the 2D case. However, the material property (3D orthotropic) created in the previous step has to be used instead of 2D orthotropic properties as in example DEFINING THE LAMINATE PROPERTY (POMPS) Predictive Engineering Document, Feel Free to Share With Your olleagues Page 39 of 66
40 The Nastran property card for 3D laminates is POMPS. Detailed information on the POMPS card is available in the Nastran User Guide. Select the Solid Laminate element/property type in the property card. By default, Femap assigns Solid element type for 3D models. The layup defined in the previous step can be assigned in the property card. The interface for the 3D laminate property card is slightly different from the 2D case. Here Ply/Stack Direction has to be assigned. For example, for the 3D laminate model the Ply/Stack Direction is specified as XZ (13). Here, X corresponds to the direction of the material angle (as defined in 2D case) and Z corresponds to the stacking direction. Unlike the 2D laminates, the 3D laminate formulation is not based on classical lamination theory. 5.5 SPEIFYING MATERIAL ANGLES The only difference between specifying material angles for a 2D case and 3D case is that the 3D model requires specifying the Ply/Stack Direction. The overall concept is still the same. 5.6 POST PROESSING THE RESULTS The image below shows the finite element mesh of the 3D laminate model. In this example, only one solid element is defined through the thickness. The thickness of the element corresponds to the total thickness of the laminate 1.56 mm. Top view Front view 1.56 mm Predictive Engineering Document, Feel Free to Share With Your olleagues Page 4 of 66
41 The 3D laminate model is analyzed with the symmetric layup configuration. The observed displacements and stresses are shown below. The displacement results are quite similar to the 2D case. The major principal stress distribution in ply 4 ( layer) is shown below. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 41 of 66
42 6. EXAMPLE 3: MODELING A SANDWIH OMPOSITE 6.1 INTRODUTION In this example, a 3D sandwich composite model is analyzed for a uniform pressure loading. The sandwich composites have a core (e.g., honeycomb, foam, etc.) sandwiched between two facesheets. Typically, the facesheets carry the majority of the inplane and bending loads while the core takes shear. A sandwich composite can be conveniently modeled using the 2D laminate layup by defining the core as one of the layers in the layup editor (shown at the end of this example). While this procedure is easy, interlaminar shear stresses (around free edges) become important in sandwich composites and 2D laminate models (based on classical lamination theory) do not account for the outofplane stresses. 6.2 REATING THE MATERIAL PROPERTY Two material models, each for the composite facesheet and core are defined. The composite facesheet is modeled as a 3D orthotropic material and the properties are shown in Table 1 (example 1). The core is modeled as an isotropic material with E = 4 GPa and ν =.25 [3]. 6.3 DEFINING THE LAYUP Defining the laminate layup for the facesheets is same as in example 2. However, it should be noted that we have two facesheets and so we have to create two solid laminate property cards, one for the top facesheet and one for the bottom facesheet. If two layups are not created separately for each of the facesheets, we will see output vectors corresponding to 8 plies only in the results set. If two layups are created, then we can see output vectors for 16 plies, 8 for the bottom facesheet and 8 for the top facesheet. 6.4 DEFINING THE PROPERTY ARDS Three property cards have to be created, two of solid laminate type for facesheets and one solid type for the core. Each of the solid laminate property cards have to be assigned to the corresponding facesheets. The material angles specification for the solid laminates is similar to the previous example. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 42 of 66
43 Facesheet ore 6.5 POST PROESSING THE RESULTS lamped boundary conditions have been applied on the sandwich composite edges and a pressure load of 1 MPa is applied on the top surface. Top view Front view Predictive Engineering Document, Feel Free to Share With Your olleagues Page 43 of 66
44 The deformation plot of the sandwich composite due to the applied pressure load is shown below. The interlaminar shear stress distribution in the core is shown below. One can mask the facesheet elements while plotting the shear stress distribution in the core. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 44 of 66
45 The bond between the core and facesheets is one of the critical regions for delamination in sandwich composites. These interlaminar shear stresses are higher at the free edges and these areas are potential regions for delamination initiation. One can compare the interlaminar shear stresses to the coretofacesheet bond shear allowable and analyze for any possible delaminations. 6.6 OTHER METHODS FOR SANDWIH OMPOSITE MODELING In this example we have developed a 3D sandwich composite model in which the facesheets and the core are modeled as solids. Other methods by which the above problem can be analyzed are: 1. 2D sandwich composite modeling in which the facesheets and the core are all 2D and can be defined in a single layup definition. This is a convenient approach however, as discussed earlier, the 2D laminate models are based on classical lamination theory and do not account for the outofplane stresses. Secondary methods are used to estimate the interlaminar stresses. Top ore Bottom 2. A mix of 2D laminates and 3D core. In this method, the facesheets can be modeled as 2D and the core can be modeled as a solid. One should be careful about defining the laminates for this configuration. Both the facesheets have to be placed at an offset of half the laminate thickness from the solid core. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 45 of 66
46 3. Using the classical plate theory to model sandwich composites. This model requires some hand calculation to be done and is complex as compared to the 2D laminate model. The Nastran property card corresponding to the plate model is the PSHELL card. In the method 1 described above, Nastran converts a POMP property into an equivalent PSHELL. So, both method 1 and method 2 should give similar results if all the properties are accurately defined. To avoid confusion, method 1 is preferred over method 2 as both are the same in terms of how Nastran interprets the property card. Alternatively, Femap has a custom tool to define a sandwich composite using the PSHELL method. One can do hand calculations and compare their values with the Femap calculated value as shown below. This custom tool for sandwich composites can be accessed from ustom tools > Honeycomb PSHELL > Honeycomb PSHELL Property. ompare your hand calculations to these Femap calculated values Predictive Engineering Document, Feel Free to Share With Your olleagues Page 46 of 66
47 7. LAMINATE FAILURE THEORIES IN FEMAP 7.1 INTRODUTION The behavior of composites is complex (as a result of heterogeneous properties) when compared to monolithic materials. Understanding the behavior of composites under extreme conditions of mechanical loading, temperature, and other environmental factors poses a great challenge. The effect of these service conditions on the composite can range from a minor loss of stiffness at microlevel to catastrophic failures at structural level. The microstructure of the composite evolves in multiple ways before evidencing measurable degradation. Typical forms of micromechanical failures include fiber breaking, matrix cracking, fiber/matrix interface debonding etc. Factors such as microcracking (typically in a matrix) are unavoidable and can be inherent in the manufactured composite part. Microcracking can result from processing the composites at high temperatures (cure cycle), due to differences of thermal conductivities/coefficients of thermal expansion between the constituents (fiber, matrix). Other forms of composite material property degradation can result from hygrothermal loading and oxidation. In this section, we will deal with the failure at ply level and not the micromechanical failures. Several failure theories have been developed to study failure envelopes of composite laminates. The failure theories that are available in Femap are discussed below. Some of these models (maximum stress theory, maximum strain theory) are based on pure comparison of observed stresses/strains in the laminate with their respective allowables. Other models such as Hill s theory, TsaiWu theory, and Hoffman s theory consider interaction of longitudinal/transverse stresses/strains to predict the failure envelope. Although failure theories can be handy to check the failure indices and decide if failure occurs in the laminate, it is important to understand the stress distribution in the model, interlaminar stresses and their effects on delamination, ABD matrices etc. 7.2 HILL S THEORY Hill s failure theory is applicable for orthotropic materials that have the same strength in tension and compression, i.e., X t = X c and Y t = Y c. Failure Index (FI) is given by: Predictive Engineering Document, Feel Free to Share With Your olleagues Page 47 of 66
48 X is allowable stress in 1direction Y is allowable stress in 2direction S is allowable stress in shear X t = Allowable tensile stress in 1direction X c = Allowable compressive stress in 1direction Y t = Allowable tensile stress in 2direction Y c = Allowable compressive stress in 2direction X = X t if σ 1 is positive or X = X c if σ 1 is negative and similarly for Y and σ 2. For the interaction term σ 1 σ 2 /X 2, X = X t if σ 1 σ 2 is positive or X = X c if σ 1 σ 2 is negative. Strength Ratio (SR) is given by, 7.3 HOFFMAN S THEORY Hoffman s theory for an orthotropic lamina in a general state of plane stress with unequal tensile and compressive strengths is given by, The failure index is obtained by evaluating the lefthand side of the above equation. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 48 of 66
49 7.4 TSAIWU THEORY The theory of strength for anisotropic materials proposed by Tsai and Wu specialized to the case of an orthotropic lamina in a general state of plane stress with unequal tensile and compressive strengths is, The failure index is obtained by evaluating the lefthand side of the above equation. F 12 is to be evaluated experimentally. By default, this term is set to zero in Femap (TsaiWu interaction term). 7.5 MAXIMUM STRAIN THEORY The maximum strain criterion has no strain interaction terms. The failure index is calculated using, X, Y, and S are allowable strains in longitudinal direction, transverse direction and inplane, respectively. A failure index for maximum stress theory (available for 3D laminate modeling) can be derived similar to maximum strain theory. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 49 of 66
50 7.6 ONSET FAILURE THEORY The Onset failure theory or the Strain Invariant Failure Theory (SIFT) is widely used in the aerospace industry. A brief overview of this failure criterion is provided in the appendix. 8. EXAMPLE 4: MODELING THE FAILURE BEHAVIOR OF OMPOSITE LAMINATES For this example, we will use the 2D laminate model from example 1. All the modeling procedure that we have done for the 2D laminate model will be supplemented by defining failure strengths of the lamina and a failure criterion. The goal is to study the failure in composite laminates and also explore the output vectors that can be handy in visualizing the failure at ply level and laminate level. 8.1 REATING THE MATERIAL PROPERTY Specify TsaiWu interaction term if you use TsaiWu failure criterion. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 5 of 66
51 8.2 DEFINING THE LAMINATE PROPERTY The laminate layup is the same as in example 1. The laminate property card is also defined in a similar manner. Additionally, we specify a failure criterion to calculate the failure indices at ply level and for the whole laminate. For this example, we will use the Hoffman s failure criterion. The bond shear allowable term is defined to predict interlaminar bond failure. If one is not interested in the interlaminar failure, this term can be left to its default value. The specification of material angles follows the same approach as in example RESULTS In this example, we are mainly interested at looking into the failure indices and evaluate the laminate and individual lamina. A uniaxial tensile load of 5 kn is applied. The contour below shows the laminate failure index and can be accessed from the output vector 66 Laminate Max Failure Index. This output vector shows the overall failure index of the laminate. A contour value (failure index) greater than or equal to 1 implies failure. Based on this information, one can assume that there are one or more layers in which the failure has occurred. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 51 of 66
52 Next, we can check the failure index output vector on a plybyply basis to find out the layers in which the failure has occurred. We can contour the output vector Lam Ply Fib Fail Index for a particular ply and then use the custom tool options Laminate Next Ply or Laminate Prev Ply and check the failure indices. Within ustom Tools > PostProcessing, Femap has an API for Laminate Envelope Failure Indices. urrently, this API generates the same output vector as 66 Laminate Max Failure Index. However, this API can be custom modified to envelop other output vectors (e.g., bond failure indices). Instead, if you are interested in manually selecting the output vectors and enveloping them to a single output vector, you can use Model > Output > Process Predictive Engineering Document, Feel Free to Share With Your olleagues Page 52 of 66
53 An example of enveloping major principal stresses in all the plies is shown below. This procedure can be followed to envelope any output vector. If the analysis has only one output set, then we can envelope the output vectors from that output set. However, if we have multiple output sets, then we need to select one or more output sets from which we would like to envelope the output vectors. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 53 of 66
54 1 2 Select this option once the other options are defined Use this option instead of manually selecting the output vector for major principal stresses in all the other plies 3 You can verify that the requested output vector is selected in all the plies Predictive Engineering Document, Feel Free to Share With Your olleagues Page 54 of 66
55 This will create new output vectors as shown below. Major Principal Stress output vector enveloped over all the plies Predictive Engineering Document, Feel Free to Share With Your olleagues Page 55 of 66
56 Other output vectors are also created which allow finding the location info (ply and element) of the maximum major principal stress. For example, from the above contour, we can see the location of the element with the maximum major principal stress. However, we do not know the respective ply that has this maximum value. The newly created output vector Envelope Location Info will have this information. One can modify the contour/criteria style to display only the max value, min value or both. Because, we are interested in max value only, required changes were done using F6 (View Options) > PostProcessing > ontour/riteria Style > Max Only. From the contour below, we can see that the maximum value of major principal stress is observed in ply 4. Maximum Major Principal Stress is observed in the output vector 1626, which corresponds to ply 4. This can be verified by checking the output vectors or from the sequence of output vectors listed below. 9. ADDITIONAL READING hapter 24: Laminates, NX Nastran User s Guide POMP and POMPS in NX Nastran Quick Reference Guide hapter 6: Element Reference Laminate Element and Solid Laminate Element in Femap User Guide I. M. Daniel and O. Ishai, Engineering Mechanics of omposite Materials, 2 nd Edition, 25. R. M. Jones, Mechanics of omposite Materials, 2 nd Edition, B. D. Agarwal, L. J. Broutman, and K. handrashekhara, Analysis and Performance of Fiber omposites, 3 rd Edition, 26. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 56 of 66
57 1. MATERIAL DATABASE This section provides material properties of some commonly used fibers, polymer resins, and fiberreinforced polymer composite materials. Typically fibers are assumed to be isotropic. However, some references also considered transversely isotropic properties (different properties in longitudinal and transverse directions) for carbon fibers. Matrix materials are typically isotropic in nature. Table 2. Mechanical properties of commonly used fibers [4] Fiber Tensile Modulus (GPa) Tensile Strength (MPa) Density (kg/m 3 ) EGlass SGlass AS4 arbon IM7 arbon Kevlar Kevlar Boron Table 3. Mechanical properties of commonly used polymer resins [5] Resin Tensile Modulus (GPa) Tensile Strength (MPa) Density (kg/m 3 ) Epoxy Polycarbonate Polyethylene Polyurethane Polyvinyl hloride Predictive Engineering Document, Feel Free to Share With Your olleagues Page 57 of 66
58 Table 4. Mechanical properties of commonly used fiberreinforced polymer composite materials Predictive Engineering Document, Feel Free to Share With Your olleagues Page 58 of 66
59 11. APPENDIX 11.1 LASSIAL LAMINATION THEORY The classical lamination theory (LT) is similar to the classical plate theory (PT), the only difference is that PT assumes that the material is isotropic, while the LT is an extension to fiberreinforced composite laminates with multiple layers resulting in complicated stressstrain relations [6]. Similar to the EulerBernoulli beam theory and the plate theory, the LT is only valid for thin laminates (span and width > 1 thinckness) with small displacements in the transverse direction. The four cornerstones of the LT are the kinematic, constitutive, force resultant, and equilibrium equations KINEMATI EQUATIONS Here, u, v, and w are the displacements of the middle plane in the x, y, and z directions. Similarly, ε x, ε y, and γ xy are the midplane strains, and ĸ x, ĸ y, and ĸ xy are the curvatures ONSTITUTIVE EQUATIONS where the subscript k indicates the k th layer counting from the top of the laminate. Predictive Engineering Document, Feel Free to Share With Your olleagues Page 59 of 66
60 RESULTANTS The terms on the left hand side are force and moment resultants EQUILIBRIUM EQUATIONS STIFFNESS MATRIES A, B, AND D The relations between the resultants (forces N and moments M) and the strains (strains ε and curvatures ĸ) are of interest in composite laminates. By replacing the stresses in the force and moment resultants with strains via the constitutive equations, we have Predictive Engineering Document, Feel Free to Share With Your olleagues Page 6 of 66
61 By applying the summation and integration operations to their respective components, the force and moment resultants can be expressed as, The above equations can be expressed as, where A is called the extensional stiffness, B is called the coupling stiffness, and D is called the bending stiffness of the laminate. The components of these three stiffness matrices are defined as follows: Predictive Engineering Document, Feel Free to Share With Your olleagues Page 61 of 66
62 Here t k is the thickness of the k th layer and is the distance from the midplane to the centroid of the k th layer UNSYMMETRI LAYUP From the classical lamination theory, we have the following relation between force/moment resultants, and the strains and curvatures. For example consider only the axial force component N x. We have, N x = A 11 ε x + A 12 ε y + A 16 γ xy + B 11 κ x + B 12 κ y + 2B 16 κ xy For an isotropic material, we have only A 11 and A 12. The remaining components A 16, B 11, B 12, and B 16 are all zero. Thus, the axial force component in an isotropic material is related to inplane strains only. However, for composite laminates, Predictive Engineering Document, Feel Free to Share With Your olleagues Page 62 of 66
QUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationA Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber
A Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber Kibong Han Mechatronics Department, Jungwon University, 85 Munmuro, Goesangun, South Korea.
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More informationUsing MATLAB to Design and Analyse Composite Laminates
Engineering, 2010, 2, 904916 doi:10.4236/eng.2010.211114 Published Online November 2010 (http://www.scirp.org/journal/eng). Using MATLAB to Design and Analyse Composite Laminates Abstract Avinash Ramsaroop,
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationStacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous Orthotropic Laminates.
49th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials 710 April 2008, Schaumburg, IL AIAA 20081940 Stacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationA SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST
A SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST P. Robinson The Composites Centre, Department of Aeronautics, Imperial College London South Kensington, London, SW7 2AZ, UK p.robinson@imperial.ac.uk
More informationModeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites
Modeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites H.E.Pettermann 1, C.Schuecker 1, D.H.Pahr 2, F.G.Rammerstorfer 2 1 Austrian Aeronautics
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationFINITE ELEMENT ANALYSIS OF A LAYERED COMPOSITE CYLINDER USING THE CONNECTION BETWEEN THE MACRO AND MICROSTRUCTURE
FINITE ELEMENT ANALYI OF A LAYERED COMPOITE CYLINDER UING THE CONNECTION BETWEEN THE MACRO AND MICROTRUCTURE A. zekrényes Research Assistant, Department of Applied Mechanics, Budapest University of Technology
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationDELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS
DELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS L Iannucci 1, M S I Shaik Dawood 1,2,3, E Greenhalgh 1 and A K Ariffin 3 1 Aeronautics Department, Imperial College London, South Kensington
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationCrashworthy Design of Composite Structures Using CAE Process Chain
0 th European LSDYNA Conference 205, Würzburg, Germany Crashworthy Design of Composite Structures Using CAE Process Chain Madhukar Chatiri, Thorsten Schuetz 2, Anton Matzenmiller 3 CADFEM GmbH, Grafing
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationFinite ElementBased Failure Models for Carbon/Epoxy Tape Composites
Finite ElementBased Failure Models for Carbon/Epoxy Tape Composites A Master Thesis Presented to The Academic Faculty by Guillaume Seon In Partial Fulfillment of the Requirements for the Degree Master
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationEXPERIMENTAL AND NUMERICAL STUDY OF THE ENERGY ABSORPTION CAPACITY OF PULTRUDED COMPOSITE TUBES
EXPERIMENTAL AND NUMERICAL STUDY OF THE ENERGY ABSORPTION CAPACITY OF PULTRUDED COMPOSITE TUBES D. Kakogiannis 1, D. Van Hemelrijck 1, J. Wastiels 1, S. Palanivelu 2, W. Van Paepegem 2, K. De Wolf 3, J.
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationOverview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling
Overview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling R. Haynes epartment of erospace Engineering, Georgia Institute of Technology 27 Ferst rive W, tlanta, G 33325, US robert.haynes@gatech.edu
More informationEffects of geometry and properties of fibre and matrix on overall. composite parameters
Int. Journal of Applied Sciences and ngineering Research, ol. 3, Issue 4, 2014 www.ijaser.com 2014 by the authors Licensee IJASR Under Creative Commons License 3.0 editorial@ijaser.com Research article
More information3D Compression Molding
Autodesk Simulation Moldflow Insight 2014 3D Compression Molding Executive summary In this work, the simulation results from a program developed for the threedimensional analysis of compression molding
More informationTESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS
TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS I. M. Daniel, J. L. Abot, and K. A. Wang Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert R. McCormick School of Engineering
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More information3. Overview of MSC/NASTRAN
3. Overview of MSC/NASTRAN MSC/NASTRAN is a general purpose finite element analysis program used in the field of static, dynamic, nonlinear, thermal, and optimization and is a FORTRAN program containing
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationRandom Vibration Analysis in FEMAP An Introduction to the Hows and Whys
Random Vibration Analysis in FEMAP An Introduction to the Hows and Whys Adrian Jensen, PE Senior Staff Mechanical Engineer Kyle Hamilton Staff Mechanical Engineer Table of Contents 1. INTRODUCTION... 4
More informationPLY WAVINESS ON INPLANE STIFFNESS OF COMPOSITE LAMINATES
PLY WAVINESS ON INPLANE STIFFNESS OF COMPOSITE LAMINATES Cimini Jr., Carlos A., and Tsai, Stephen W. 2 Department of Mechanical Engineering, Federal University of Minas Gerais Av. Antônio Carlos, 6627
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationMODELLING OF THE THERMOMECHANICAL PROPERTIES OF WOVEN COMPOSITES DURING THE CURE
TH 9 TH INTRNATIONAL ONFRN ON OMPOSIT MATRIALS MODLLING OF TH THRMOMHANIAL PROPRTIS OF WOVN OMPOSITS DURING TH UR L. Khoun,, K.S. hallagulla,, P. Hubert Department of Mechanical ngineering, McGill University,
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More information*MAT_PAPER and *MAT_COHESIVE_PAPER: Two New Models for Paperboard Materials
14 th International LSDYNA Users Conference Session: Constitutive Modeling *MAT_PAPER and *MAT_COHESIVE_PAPER: Two New Models for Paperboard Materials Jesper Karlsson 1, Mikael Schill 1, Johan Tryding
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationInterlaminar fracture characterization in composite materials by using acoustic emission
5th International Symposium on NDT in Aerospace, 1315th November 2013, Singapore Interlaminar fracture characterization in composite materials by using acoustic emission Ian SILVERSIDES 1, Ahmed MASLOUHI
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationChapter 5. Vibration Analysis. Workbench  Mechanical Introduction ANSYS, Inc. Proprietary 2009 ANSYS, Inc. All rights reserved.
Workbench  Mechanical Introduction 12.0 Chapter 5 Vibration Analysis 51 Chapter Overview In this chapter, performing free vibration analyses in Simulation will be covered. In Simulation, performing a
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationANSYS Mechanical Basic Structural Nonlinearities
Lecture 4 Rate Independent Plasticity ANSYS Mechanical Basic Structural Nonlinearities 1 Chapter Overview The following will be covered in this Chapter: A. Background Elasticity/Plasticity B. Yield Criteria
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationFailure from static loading
Failure from static loading Topics Quiz /1/07 Failures from static loading Reading Chapter 5 Homework HW 3 due /1 HW 4 due /8 What is Failure? Failure any change in a machine part which makes it unable
More informationElastic parameters prediction under dynamic loading based on the. unit cell of composites considering end constraint effect
Elastic parameters prediction under dynamic loading based on the unit cell of composites considering end constraint effect Wang Meng 1,, Fei Qingguo 1,, Zhang Peiwei 1, (1. Institute of Aerospace Machinery
More informationInternational Journal of Advanced Engineering Technology EISSN
Research Article INTEGRATED FORCE METHOD FOR FIBER REINFORCED COMPOSITE PLATE BENDING PROBLEMS Doiphode G. S., Patodi S. C.* Address for Correspondence Assistant Professor, Applied Mechanics Department,
More informationREPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 REPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More informationJournal of Composite Materials. Behaviour of hollow pultruded GFRP square beams with different shear spantodepth ratios
Behaviour of hollow pultruded GFRP square beams with different shear spantodepth ratios Journal: Manuscript ID: Draft Manuscript Type: Original Manuscript Date Submitted by the Author: n/a Complete List
More informationMECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS
MECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS This paper provides a preliminary stress analysis of a carbon reinforced layered cylinder such as would be found in a yacht mast. The cylinder is
More information9 Strength Theories of Lamina
9 trength Theories of Lamina 9 TRENGTH O ORTHOTROPIC LAMINA or isotropic materials the simplest method to predict failure is to compare the applied stresses to the strengths or some other allowable stresses.
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationFinite Element Modelling with Plastic Hinges
01/02/2016 Marco Donà Finite Element Modelling with Plastic Hinges 1 Plastic hinge approach A plastic hinge represents a concentrated postyield behaviour in one or more degrees of freedom. Hinges only
More informationAPPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN
28 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES APPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN Tuyen Tran*, Dan Simkins**, Shen Hin Lim*,
More informationFinite Element Analysis Prof. Dr. B. N. Rao Department of Civil Engineering Indian Institute of Technology, Madras. Module  01 Lecture  11
Finite Element Analysis Prof. Dr. B. N. Rao Department of Civil Engineering Indian Institute of Technology, Madras Module  01 Lecture  11 Last class, what we did is, we looked at a method called superposition
More informationLecture #10: Anisotropic plasticity Crashworthiness Basics of shell elements
Lecture #10: 1510735: Dynamic behavior of materials and structures Anisotropic plasticity Crashworthiness Basics of shell elements by Dirk Mohr ETH Zurich, Department of Mechanical and Process Engineering,
More informationS. Srinivasan, Technip Offshore, Inc., Houston, TX
9 th ASCE Specialty Conerence on Probabilistic Mechanics and Structural Reliability PROBABILISTIC FAILURE PREDICTION OF FILAMENTWOUND GLASSFIBER Abstract REINFORCED COMPOSITE TUBES UNDER BIAXIAL LOADING
More information14. LSDYNA Forum 2016
14. LSDYNA Forum 2016 A Novel Approach to Model Laminated Glass R. Böhm, A. Haufe, A. Erhart DYNAmore GmbH Stuttgart 1 Content Introduction and Motivation Common approach to model laminated glass New
More informationUSE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION ARJUN KOTHIDAR
USE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION By ARJUN KOTHIDAR A thesis submitted in partial fulfillment of the requirements for the degree
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationAdvances in Micromechanics Modeling of Composites. Structures for Structural Health Monitoring. Albert Moncada
Advances in Micromechanics Modeling of Composites Structures for Structural Health Monitoring by Albert Moncada A Dissertation Presented in Partial Fulfillment of the Requirements for the Degree Doctor
More informationAim of the study Experimental determination of mechanical parameters Local buckling (wrinkling) Failure maps Optimization of sandwich panels
METNET Workshop October 1112, 2009, Poznań, Poland Experimental and numerical analysis of sandwich metal panels Zbigniew Pozorski, Monika ChudaKowalska, Robert Studziński, Andrzej Garstecki Poznan University
More information